High Strength Glass-Ceramics Fabricated With Coal High strength glass-ceramics were fabricated with
Embed Size (px)
Transcript of High Strength Glass-Ceramics Fabricated With Coal High strength glass-ceramics were fabricated with
Chen P* Department of Material Science and Engineering, Shaanxi University of Science and Technology, China
*Corresponding author: Chen P, College of Material Science and Engineering, Shaanxi University of Science and Technology, Xi’an, Shaanxi, China (710021)
Submission: November 09, 2017 Published: April 13, 2018
High Strength Glass-Ceramics Fabricated With Coal Gangue as Main Raw Materials
Introduction Glass-ceramics are attractive materials used in various
applications, such as building materials, cooking ceramics, machinable ceramics, bio-ceramics, optical materials, etc [1,2]. High strength and lightweight are first requirement for some applications. From a point of raw material, utilizing the industrial solid wastes with high contents of silica and alumina is a main direction of developing the glass-ceramics because of low cost and high product performance.
Since the main constituents of glass-ceramics are SiO2, Al2O3, CaO and/or MgO, many inorganic wastes are potential starting materials. Currently, various wastes have been used, such as, slags, coal ash, incinerator ash, and waste glass, and shell, oil shale ash and phosphorous fertilizer. Coal gangue as a type of industrial solid waste is widely used to produce cement , ceramics [4,5], refractory brick , zeolite , lightweight aggregate , and so on. A very large amount of the coal gangue is produced in coal production. The amount produced in china is reached above several million tones, and increases about one millions tones per year.
However, the comprehensive utilization rate of the coal gangue is limited. To prevent air and river from pollution and save resource, the efficient management and full utilization of the coal gangue are urgent. The coal gangue has a high alumina content of ~30 wt% and a high silica content of ~62 wt%, and so is suitable for fabrication of the high strength glass-ceramics. In this work, we report the fabrication and the property of the glass-ceramics with the coal gangue as a main raw material.
Experimental Procedure The coal gangue was used as main raw materials. Bauxite was
used to increase the alumina content in the glass-ceramics. Clay was used as an adhesive and to improve formability of slurry. In addition, small amounts of steatite and limestone were used as additives; and BaCO3, MnCO3, and MgCO3 were used as mineralizers. The sodium tripolyphosphate (STPP) and methyl cellulose (CMC) was used as a water reducer to decrease viscosity of the slurry. The chemical composition of the raw materials is listed in Table 1.
Aspects in Mining & Mineral ScienceC CRIMSON PUBLISHERSWings to the Research
128Copyright © All rights are reserved by Chen P. Volume 1 - Issue - 5
High strength glass-ceramics were fabricated with coal gangue as main raw material. The effects of the utilization rate of the coal gangue, mineral additives, mineralization agents, forming process, and sintering process on the properties of the glass-ceramics were studied. The optimal utilization rate of coal gungue is 55 wt% when the utilization rate of another mineral material bauxite is 35 wt%. The glass-ceramics showed a main crystal phase of mullite. BaCO3 and MnCO3 codoping and cosubstitution as mineralization agents obviously enhanced the properties of the glass-ceramics. The strength of 148.36-156.12 MPa, water absorption of 0.17-0.02%, and density of 2.66-2.68g/cm3 were achieved for the glass-ceramics. By optimization experiments, reasonable and optimal processing parameters of forming and sintering were also determined.
Keywords: Coal cangue; Glass-Ceramics; Process optimization; Mechanics property
Table 1: The composition of the raw materials (wt %).
Raw Material SiO2 Al2O3 CaO MgO Fe2O3 TiO2 K2O Na2O
Coal gangue 62.5 20.8 2.12 4.83 3.14 0.83 3.12 3.17 0.7
bauxite 7.25 76.25 1 1 1.5 1.5 0 0 11.5
clay 41.03 37.71 2.66 0.46 0.14 0.14 0.68 0.54 14.18
limestone 1.51 0 55.28 0 0 0 0 0 43.22
steatite 62.82 1.03 2.06 31.93 0.1 0 0 0 2.06
http://crimsonpublishers.com/amms/index.php http://crimsonpublishers.com/amms/index.php http://crimsonpublishers.com/index.php
Aspects Min Miner Sci
Copyright © Chen P
129 How to cite this article: Chen P. High Strength Glass-Ceramics Fabricated With Coal Gangue as Main Raw Materials. Aspects Min Miner Sci. 1(5). AMMS.000522.2018. DOI: 10.31031/AMMS.2018.01.000522
Volume 1 - Issue - 5
Table 2: The basic prescriptions of samples (wt %).
Bauxite Clay Steatite Limestone
1# 60 30 5 3 2
2# 55 35 5 3 2
3# 50 40 5 3 2
4# 45 45 5 3 2
5# 40 50 5 3 2
Mullite (Al6Si2O13) generally has high strength and so was designed as main crystal phase. Combine with utilization rate of the coal gangue; the basic prescriptions were designed as listed in Table 2.
Typical processes for fabrication of the glass-ceramics are mentioned below: the raw materials were first mixed according to the designed prescriptions. The mixtures were filtered through 10 mesh, wet-milled at ratio of raw materials: ball: water=1: 2.5: (0.3- 0.5) for 15-25min and then filtered through 120 mesh (Aparture: 0.045mm, ASTM). Subsequently, as treated raw materials were dried at 50-70 ⁰C for 3-5h, the each of the dried samples with a weight of ~200g were taken, and 5g STPP and 5g CMC were added into each sample. By further ball-milling with appropriate water for 12 min, the slurry was filtered through 80 mesh (Aparture: 0.180mm, ASTM). Residue on sieve is ~0.1%. After drying at 50- 70 ⁰C for 3-5h, the powder was ground and then filtered through 55 mesh (Aparture: 0.280mm, ASTM). The obtained fine powders
were prilled by spraying water and stirring. The prilled grains were filtered through 20 mesh (Aparture: 0.850mm, ASTM). The fine grains under the sieve were re-sprayed with water with constant stirring and then processed to shape required for strength measurement. The formed samples were then pressed at 25-35 MPa and dried at 50-100 ⁰C for 24h. The large grains on the sieve were dried at 80 ⁰C for 4 h. The dried samples and large grains were finally heated at a heating rate of 5-10 ⁰C/ min to 1290-1430 ⁰C and calcined for 30-90min.
The structural phase of the glass-ceramics was identified at room temperature using X-Ray diffractometer (XRD, CuKα1, λ=0.15406nm, Model No. D/Max-2200PC, Rigaku, Japan). The morphology of the glass-ceramics was analyzed by scanning electron microscopy (SEM, Model No: S-570, Japan). The flexural strength of the glass-ceramics was measured by a strength tester (Model No: 401/3, Germany). The water absorbance (Aw) of the grain glass-ceramics was calculated by following equation:
h d w
W W A
Where Wd is weight of appropriate amount of the grains after dried at 110 ⁰C for 3h, Wh is weight of the above dried grains after soaked in water at room temperature for 36h. The density of the grain glass-ceramics (d) was calculated by equation:
Where m0 is mass of the appropriate amount of the grains after drying at 105-110 ⁰C for 3h, m1 is mass of the grains immersing in water at room temperature.
Results and Discussion
Figure 1: Variations of (a) flexural strength and (b) water absorbance of the glass-ceramics fabricated with basic prescription 1−5# with sintering temperature (Sintering time: 30min; milling time: 20min; forming pressure: 30MPa).
Table 3: The prescriptions of samples containing various mineralizers (wt %).
No Coal Gangue Bauxite Clay Steatite Limestone BaCO3 MnCO3 MgCO3
6# 55 35 5 3 2 3 0 0
7# 55 35 5 3 2 0 3 0
8# 55 35 5 3 2 0 0 3
9# 55 35 5 3 2 3 3 0
130 How to cite this article: Chen P. High Strength Glass-Ceramics Fabricated With Coal Gangue as Main Raw Materials. Aspects Min Miner Sci. 1(5). AMMS.000522.2018. DOI: 10.31031/AMMS.2018.01.000522
Aspects Min Miner Sci
Copyright © Chen P
Volume 1 - Issue - 5
10# 55 35 5 3 2 3 0 3
11# 55 35 5 3 2 0 3 3
12# 51 33 5 3 2 3 3 -
To select reasonable proportion of the coal gangue, five samples with basic prescriptions (Table 2) were first tested. Figure 1 shows variations of strength and water absorbance of glass-ceramics fabricated with different coal gangue contents as a function of sintering temperature. The glass-ceramics fabricated with prescription 2# shown a maximal strength and minimal water absorbance in the sintering temperature range of 1290-1430 ⁰C. Therefore, the prescription 2# was further studied by adding various mineralizers. Table 3 lists the new prescriptions. In which, the prescription 12# was made up by replacing coal gangue and bauxite with BaCO3 and MnCO3. Figure 2-4 illustrate the properties of the glass-ceramics formed at press of 30 MPa and sintered at different temperatures for 30min. BaCO3 and MnCO3 codoping (prescription 9#) leads to better effects with a minimal water absorption (0.17%), maximal flexural strength (148.36 MPa) and density (2.66g/ cm3). Furthermore, the BaCO3 and MnCO3 cosubstitution leads to an optimal effect. That is, minimal water absorption (0.02%), maximal flexural strength (156.12 MPa) and density (2.68g/cm3) are achieved. Optimal sintering temperature for these samples is 1360. The chemical composi